NOVELTY - Anti-reflection coating is prepared by mixing decamethyl acryloyloxypropyl cage-type silsesquioxane:octaaminophenyl cage-type silsesquioxane with mass ratio of 1:1-50:1 to obtain bottom layer spin-coating material, adding methanol:acetone mixed solvent with mass ratio of 1:1 and Aza-Michael addition reaction catalyst, mixing to obtain bottom layer spin-coating solution, placing in transparent substrate center, 1st spin-coating with spin-coating device to obtain 80-90 nm thick uniform transparent bottom layer thin film, placing in vacuum oven, and pre-solidifying at 80 degrees C for 15-30 minutes.    USE - Preparation of anti-reflection coating for e.g. display, camera lens, glasses, and solar energy cell (all claimed).    ADVANTAGE - Anti-reflection coating has improved anti-reflection performance, heat resistance, and corrosion resistance, and preparation is simple and convenient.    DETAILED DESCRIPTION - Anti-reflection coating is prepared by mixing decamethyl acryloyloxypropyl cage-type silsesquioxane:octaaminophenyl cage-type silsesquioxane with mass ratio of 1:1-50:1 to obtain bottom layer spin-coating material, adding methanol:acetone mixed solvent with mass ratio of 1:1 and Aza-Michael addition reaction catalyst, mixing to obtain bottom layer spin-coating solution, placing in transparent substrate center, 1st spin-coating with spin-coating device to obtain 80-90 nm thick uniform transparent bottom layer thin film, placing in vacuum oven, pre-solidifying at 80 degrees C for 15-30 minutes to obtain bottom coating, adding fluorinated acrylate monomer and benzoyl peroxide in reactor, reacting at 80-90 degrees C for 30-60 minutes obtain fluorinated acrylate prepolymer, adding octamethyl acryloyloxypropyl cage-type silsesquioxane, dissolving using ultrasound to obtain surface layer spin-coating solution, placing on center of bottom coating, 2nd spin-coating using spin-coating device to obtain 100-110 nm thick uniform transparent surface layer thin film, placing in vacuum oven, co-curing at 80 degrees C for 6-12 hours, heating to 150 degrees C, and co-curing for 12-24 hours.    DESCRIPTION OF DRAWING(S) - The drawing shows an atomic force microscopy image of anti-reflection coating.